# Lattice constant

(Redirected from Lattice matching)
Unit cell definition using parallelopiped with lengths a, b, c and angles between the sides given by α,β,γ[1]

The lattice constant, or lattice parameter, refers to the physical dimension of unit cells in a crystal lattice. Lattices in three dimensions generally have three lattice constants, referred to as a, b, and c. However, in the special case of cubic crystal structures, all of the constants are equal and we only refer to a. Similarly, in hexagonal crystal structures, the a and b constants are equal, and we only refer to the a and c constants. A group of lattice constants could be referred to as lattice parameters. However, the full set of lattice parameters consist of the three lattice constants and the three angles between them.

For example the lattice constant for a common carbon diamond is a = 3.57 Å at 300 K. The structure is equilateral although its actual shape cannot be determined from only the lattice constant. Furthermore, in real applications, typically the average lattice constant is given. Near the crystal's surface, lattice constant is affected by the surface reconstruction that results in a deviation from its mean value. This deviation is especially important in nano-crystals since surface to nano-crystal core ratio is large.[2] As lattice constants have the dimension of length, their SI unit is the meter. Lattice constants are typically on the order of several angstroms (i.e. tenths of a nano-metre). Lattice constants can be determined using techniques such as X-ray diffraction or with an atomic force microscope.

In epitaxial growth, the lattice constant is a measure of the structural compatibility between different materials. Lattice constant matching is important for the growth of thin layers of materials on other materials; when the constants differ, strains are introduced into the layer, which prevents epitaxial growth of thicker layers without defects.

## Lattice matching

Matching of lattice structures between two different semiconductor materials allows a region of band gap change to be formed in a material without introducing a change in crystal structure. This allows construction of advanced light-emitting diodes and diode lasers.

For example, gallium arsenide, aluminium gallium arsenide, and aluminium arsenide have almost equal lattice constants, making it possible to grow almost arbitrarily thick layers of one on the other one.

Typically, films of different materials grown on the previous film or substrate are chosen to match the lattice constant of the prior layer to minimize film stress.

An alternative method is to grade the lattice constant from one value to another by a controlled altering of the alloy ratio during film growth. The beginning of the grading layer will have a ratio to match the underlying lattice and the alloy at the end of the layer growth will match the desired final lattice for the following layer to be deposited.

The rate of change in the alloy must be determined by weighing the penalty of layer strain, and hence defect density, against the cost of the time in the epitaxy tool.

For example, indium gallium phosphide layers with a band gap above 1.9 eV can be grown on gallium arsenide wafers with index grading.

## List of Lattice Constants at 300K

Material Lattice Constant (Å) Crystal Structure Ref
C (diamond) 3.567 Diamond (FCC) [3]
C (graphite) 2.461(a); 6.708(c) Hexagonal
Si 5.431 Diamond (FCC) [4]
Ge 5.658 Diamond (FCC) [4]
AlAs 5.6605 Zinc blende (FCC) [4]
AlP 5.4510 Zinc blende (FCC) [4]
AlSb 6.1355 Zinc blende (FCC) [4]
GaP 5.4505 Zinc blende (FCC) [4]
GaAs 5.653 Zinc blende (FCC) [4]
GaSb 6.0959 Zinc blende (FCC) [4]
InP 5.869 Zinc blende (FCC) [4]
InAs 6.0583 Zinc blende (FCC) [4]
InSb 6.479 Zinc blende (FCC) [4]
MgO 4.212 Rocksalt (FCC) [1]
SiC 3.086(a); 10.053 (c) Wurtzite [4]
CdS 5.8320 Zinc blende (FCC) [3]
CdSe 6.050 Zinc blende (FCC) [3]
CdTe 6.482 Zinc blende (FCC) [3]
ZnO 4.580 Rocksalt (FCC) [3]
ZnS 5.420 Zinc blende (FCC) [3]
PbS 5.9362 Rocksalt (FCC) [3]
PbTe 6.4620 Rocksalt (FCC) [3]
BN 3.6150 Zinc blende (FCC) [3]
BP 4.5380 Zinc blende (FCC) [3]
CdS 4.160(a); 6.756(c) Wurtzite [3]
ZnS 3.82(a); c=6.26(c) Wurtzite [3]
AlN 3.112(a); 4.982(c) Wurtzite [4]
GaN 3.189(a); 5.185(c) Wurtzite [4]
InN 3.533(a); 5.693(c) Wurtzite [4]
LiF 4.03 Rocksalt
LiCl 5.14 Rocksalt
LiBr 5.50 Rocksalt
LiI 6.01 Rocksalt
NaF 4.63 Rocksalt
NaCl 5.64 Rocksalt
NaBr 5.97 Rocksalt
NaI 6.47 Rocksalt
KF 5.34 Rocksalt
KCl 6.29 Rocksalt
KBr 6.60 Rocksalt
KI 7.07 Rocksalt
RbF 5.65 Rocksalt
RbCl 6.59 Rocksalt
RbBr 6.89 Rocksalt
RbI 7.35 Rocksalt
CsF 6.02 Rocksalt
CsCl 4.123 Cesium Chloride
CsI 4.567 Cesium Chloride
Al 4.046 FCC [5]
Fe 2.856 BCC [5]
Ni 3.499 FCC [5]
Cu 3.597 FCC [5]
Mo 3.142 BCC [5]
Pd 3.859 FCC [5]
Ag 4.079 FCC [5]
W 3.155 BCC [5]
Pt 3.912 FCC [5]
Au 4.065 FCC [5]
Pb 4.920 FCC [5]
TiN 4.249 Rocksalt
ZrN 4.577 Rocksalt
HfN 4.392 Rocksalt
VN 4.136 Rocksalt
CrN 4.149 Rocksalt
NbN 4.392 Rocksalt
TiC 4.328 Rocksalt [6]
ZrC0.97 4.698 Rocksalt [6]
HfC0.99 4.640 Rocksalt [6]
VC0.97 4.166 Rocksalt [6]
NC0.99 4.470 Rocksalt [6]
TaC0.99 4.456 Rocksalt [6]
Cr3C2 11.47(a); 5.545(b); 2.830(c) Orthorombic [6]
WC 2.906(a);2.837(c) Hexagonal [6]
ScN 4.52 Rocksalt [7]
LiNbO3 5.1483(a);13.8631(c) Hexagonal [8]
KTaO3 3.9885(a) Cubic perovskite [8]
BaTiO3 3.994(a);4.034(c) Tetragonal perovskite [8]
SrTiO3 3.98805(a) Cubic perovskite [8]
CaTiO3 5.381(a);5.443(b);7.645(c); Orthorhombic perovskite [8]
PbTiO3 3.904(a);4.152(c); Tetragonal perovskite [8]
EuTiO3 7.810(a) Cubic perovskite [8]
SrVO3 3.838(a) Cubic perovskite [8]
CaVO3 3.767(a) Cubic perovskite [8]
BaMnO3 5.673(a);4.71(c) Hexagonal [8]
CaMnO3 5.27(a);5.275(b);7.464(c); Orthorhombic perovskite [8]
SrRuO3 5.53(a);5.57(b);7.85(c); Orthorhombic perovskite [8]
YAlO3 5.179(a);5.329(b);7.37(c); Orthorhombic perovskite [8]

## References

1. ^ Unit cell definition using parallelepiped with lengths a, b, c and angles between the sides given by α,β,γ
2. ^ Mudar A. Abdulsattar, Solid State Sci. 13, 843 (2011).
3. "Lattice Constants". Argon National Labs (Advanced Photon Source). Retrieved 19 October 2014.
4. "Semiconductor NSM". Retrieved 19 October 2014.
5. Davey, Wheeler (1925). "PRECISION MEASUREMENTS OF THE LATTICE CONSTANTS OF TWELVE COMMON METALS". Physical Reviews 25: 753. doi:10.1103/PhysRev.25.753.
6. Toth, L.E. (1967). Transition Metal Carbides and Nitrides. New York: Academic Press.
7. ^ Saha, B. (2010). "Electronic structure, phonons, and thermal properties of ScN, ZrN, and HfN: A first-principles study". Journal of Applied Physics 107: 033715. doi:10.1063/1.3291117.
8. Goodenough, J.B.; Longo, M. "3.1.7 Data: Crystallographic properties of compounds with perovskite or perovskite-related structure, Table 2 Part 1". SpringerMaterials - The Landolt-Börnstein Database.